Vijay Kumar Thakur and A S Singha258lose is principally responsible for strength of natural fibrebecause of its specific properties such as high degree ofpolymerization and linear orientation. Mechanical proper-ties of these fibres are dependent on the cellulose contentin the fibre, the degree of polymerization of the celluloseand the micro fibril angle. Fibres with higher cellulosecontent, higher degree of polymerization and a lowermicrofibrillar angle exhibit higher tensile strength andmodulus. These fibres exhibit variations in mechanicalproperties both along the length of an individual fibre andbetween fibres. Hemicelluloses act as a matrix for thecellulose. It is supposed to act as a link between thefibrous cellulose and the amorphous lignin. Lignin is aphenolic compound that holds the fibres together. Ligninacts as a stiffening agent for the cellulose moleculeswithin the fibre cell walls. All three cell wall compo-nents contribute in different extents to the strength offibre.1.2 MatrixMatrix is a material which encapsulates two or morethan two components in itself. In case of natural fibre-reinforced composite material, matrix binds the fibrestogether. It transfers applied load to these fibres and alsoprotects these fibres from harmful environmental effects.Various types of materials are generally used as matrixmaterial such as metal matrix, ceramic matrix, carbongraphite matrix, glass matrix and polymer matrix. Amongthese, polymer matrices are currently being used to alarger extent because of their enormous advantages (Rayet al 2001; Nakagaito and Yano 2004, 2005; Majumdarand Adhikari 2005; Panthapulakkal et al 2006). Therequirements for the matrix in Pine needle reinforcedpolymer composite are: (i) to bind the fibres together, andprotect their surfaces from damage during fabrication inthe service of life of the composite, (ii) melting pointshould be lower than the degradation temperature of thefibres, (iii) to keep the fibres dispersed and separated so asto avoid any catastrophic propagation of cracks and sub-sequent failure, (iv) to transfer stresses to the fibres effi-ciently by adhesion and/or friction, when the composite isunder load, (v) to be thermally compatible with the rein-forcement and (vi) to be chemically compatible with thefibres over a long period.Common methods for manufacturing natural fibre rein-forced polymer composites are compression molding andextrusion (Bledzki and Gassan 1999; Singha and Thakur2008a, b). Himachal Pradesh is the hilliest state in India.Pine trees are abundantly found in Himachal Pradesh.Pine needles are the main cause of fire during summerseason when trees shed their needles. This article examinesthe feasibility of raw Pine needle as reinforcingmaterial for producing Pine needle reinforced polymercomposites.2. Experimental2.1 Materials and methods2.1a Matrix polymer: Urea, formaldehyde solution andsodium hydroxide were kindly supplied by QualigensChemicals Ltd. and were used as received. Resin synthe-sized from urea and formaldehyde was used as matrixpolymer.2.1b Reinforcing filler: The ligno-cellulosic materialused as the reinforcing filler in the composite was Pineneedles collected from NIT Campus Hamirpur (HP). Thefibres were washed thoroughly with distilled water anddried in an air oven at 70°C for 12 h and in vacuum ovenat 63°C for 3 h before preparation of composites. Thisfibre was used in three forms as shown here: (i) Particlereinforcement: Pine needles were grinded to a powderand filtered through a sieve of pore size, 200 μm, (ii)Short-fibre reinforcement: Pine needles were choppedinto 3 mm size. This fibre was used as short fibre and (iii)Long fibre reinforcement: Pine needles were chopped into6 mm size. This fibre was used as long fibre.2.2 Instruments usedWeights of the samples were taken on Shimadzu makeelectronic balance (LIBROR AEG-220). Curing of differentsamples prepared was done on compression moldingmachine (SANTECH INDIA Ltd). Testing of samples fortensile and compressive strengths were done on Compu-terized Universal Testing Machine (HOUNSFIELDH25KS) and wear testing was done on Wear & FrictionMonitor (DUCOM-TR-20L). Morphological (SEMmicrograph) and thermal studies (TGA/DTA, DTG) werecarried out on LEO 435VP make SEM and on TGAmachine LINSEIS, L 81-11 make, respectively.2.3 Synthesis of urea–formaldehyde resinUrea–formaldehyde resin was synthesized by the standardmethod developed in our laboratory described somewhereelse (Singha and Thakur 2008b). The resin samples werethen cured at 130°C in compression molding machine. Thecured samples were then subjected to various mechanical,thermal and morphological studies.2.4 Mechanism of polymerization reactionThe polymerization reaction between urea and formalde-hyde is supposed to take place in two steps (Singha andThakur 2008b). First step involves the reaction betweenurea and formaldehyde to form methylol urea. Since ureais tetra functional, initial reaction may lead to the forma-
Natural fibres-based polymers 259Figure 1. (A) Formation of methylol derivatives of urea and (B) condensation of methylol urea byelimination.tion of tetra methylol derivative of urea (as shown in fig-ure 1A). However, slightly alkaline medium (pH of 7–8)control the reaction and favour the formation of dimethy-lol urea. Since these methylol ureas are non adhesive innature so condensation does not take place. However, thecondensation takes place in acidic medium. Therefore,the reaction is carried out at 80–90°C and reaction speedis controlled by the acidity of the medium (pH 5⋅5–6). Asthe reaction proceeds larger molecules with cross linkedstructures are formed. At the requisite level, the reactionis arrested by neutralization (pH 7⋅5–8). The condensa-tion is closely watched and controlled at the stages ofproduction because if the reaction is allowed to continue,cross-linking may lead to gelatization of the resin. Underacidic conditions, methylol urea condenses by elimina-tion of water between either of four steps (as shown infigure 1B).2.5 Synthesis of polymer biocompositesNatural fibre reinforced composites were prepared byutilizing Pine needles in three different forms as dis-cussed below:2.5a Particle reinforced composites: Pine needlesgrinded to a powder of pore size, 200 μm, were mixedwith specific amount of resin by suitable loading (1 : 0⋅1).Curing of samples was done in compression molding ma-chine at 130°C and were further subjected to differentstudies.2.5b Short-fibre reinforced composites: Pine needleswere chopped into 3 mm size and mixed with the knownweight of UF resin. After proper mixing the curing ofsamples was carried out at 130°C in compression mold-ing machine.2.5c Long fibre reinforced composites: Pine needleswere chopped into 6 mm length and mixed with weighedamount of resin. Curing of samples was done as descri-bed above.2.6 Study of mechanical properties of various samples2.6a Tensile strength test: The tensile strength test wasconducted on ASTM made Computerized Universal Test-
Vijay Kumar Thakur and A S Singha260ing Machine (HOUNSFIELD H25KS). The sample of100 mm length was clamped into the two jaws of themachine. Each end of the jaws covered 20 mm of thesample. Tensile strength was deliberated over the rest of60 mm gauze length. Reading of the tensile strengthtest instrument for Newton force and extension was ini-tially set to zero. The test was conducted at the constantstrain rate of the order of 10 mm/min. Tensile stresswas applied till the failure of the sample and load-extension curve was obtained. Each sample was testedseven times.2.6b Compressive strength test: Compression strengthof samples was also performed on ASTM made Comput-erized Universal Testing Machine (HOUNSFIELDH25KS). Composite sample was held between the twoplatforms and the strain rate was fixed at 10 mm/minwhereas the total compression range was 7⋅5 mm. Thecompression stress was applied till the failure of sample.Total compression per unit force was noted.2.6c Flexural strength test: Flexural strength of sampleswas also tested on Computerized Universal Testing Ma-chine. The three-point bend flexural test was conductedin accordance with standard ASTM D method.2.6d Wear test: The wear test of the testing samplewas conducted according to Wear & Friction Monitor(DUCOM-TR-20L). The disc was cleaned with emerypaper and it was fixed at 500 rpm. The inner diameter ofsteel disc was 80 mm. Initial weight of the sample wasnoted and the sample pin was fixed in the jaws of weartesting machine. Then machine was set to display zerowear and friction. The samples were then tested withdifferent loads varying from 1–3 kg. For each load themachine was allowed to run for 15 min and the readingswere recorded. After 15 min the sample was taken outfrom the machine and weighed again. The loss in weightdue to abrasion was calculated and this weight loss wasused as the measure of wear.2.7 Thermal and morphological studiesThermal analysis of materials gives us information abouttheir thermal stability. The thermal analysis comprises ofvarious methods such as thermogravimetric analysis(TGA)/differential thermal analysis (DTA), derivativethermogravimetry (DTG) etc. Thermogravimetric analysis(TGA) and differential thermal analysis (DTA) studies ofsamples were carried out in nitrogen atmosphere on athermal analyser at a heating rate of 10°C/min. Morpho-logical analysis of different samples was carried out bystudying SEM micrographs. These SEM micrographsof the samples give us information about the morphologyof the resin and its respective biocomposite. Thesemicrographs clearly show the difference between loadedand unloaded matrix.3. Results and discussionEvaluation of mechanical properties of natural fibre rein-forced composite materials is an important tool in thestudy of the behaviour of these composite materials. Ithas been proved to be an efficient method in studying thebehaviour of the materials under various conditions oftension, compression of fibre reinforced composites andits role in determining the mechanical properties.Mechanical properties of natural fibre reinforced compo-sites principally depend on the (i) nature of the matrixmaterial and (ii) distribution and orientation of the rein-forcing fibres.3.1 Optimization of urea–formaldehyde resinOptimization of urea–formaldehyde resin has been doneby evaluating optimal mechanical properties such as tensilestrength, compressive strength, wear resistance etc(Singha and Thakur 2008b). In case of tensile strengthtest it has been observed that U–F samples of ratio 1 : 2⋅5bear more load at a particular applied load as compared tosamples of other ratios. This ratio (1 : 2⋅5) could bear aload of 128⋅125 NF with an extension of 1⋅84 mm asshown in figure 2A. On the other hand, samples of otherratios bear low loads. In compressive strength test it isevident from figure 2B that the samples of ratio 1 : 2⋅5could bear a load of 991 N at a compression of 3⋅51 mmwhile samples of other ratios bear fewer loads. It isevident from figure 2C that the samples of ratio 1 : 2⋅5could bear a maximum load of 59 N at a deflection of0⋅776 mm.In wear resistance test it has been observed that it isclear that the wear rate of samples of ratio 1 : 2⋅5 was less ascompared to any other samples (figure 1C). Loss of mate-rial was due to abrasion and friction of samples with disc.3.2 Effect of reinforcement on mechanical properties ofU–F based biocomposites3.2a Tensile strength: It has been observed that com-posites with particle reinforcement showed more tensilestrength which was followed by short fibre and long fibrereinforced composites (figures 3A–C). It is clear fromfigures 3A–C that the samples of (i) particle reinforcedcomposite could bear a load of 244⋅5 N at an extension of1⋅91 mm, (ii) short fibre reinforced composite could beara load of 200⋅5 N at an extension of 1⋅95 mm and (iii)long fibres reinforced composite could bear a load of191⋅5 N at an extension of 1⋅97 mm.
Natural fibres-based polymers 261Figure 2. Tensile/compression strength/flexural strength and wear resistance curve of UF resin(A, B, C and D).Figure 3. Tensile strength curves of P–Rnf/SF–Rnf and LF–Rnf composites (A, B and C).3.2b Compressive strength: Compressive strength ofUF resin matrix has been found to increase when rein-forced with Pine needles. It has been found that with parti-cle reinforcement, compressive strength increases to amuch more extent than short and long fibre reinforcement(figures 4A–C). It is clear that the samples of (i) particlereinforced composite could bear a load of 1895⋅5 N witha compression of 3⋅51 mm, (ii) short fibre reinforcedcomposite could bear a load of 1775 N with a compres-sion of 3⋅53 mm and (iii) long fibre reinforced compositecould bear a load of 1685 N with a compression of3⋅586 mm.3.2c Flexural strength: Flexural strength of Pineneedles reinforced composites also follows the same trendas in case of tensile and compressive strength. It is clearfrom figures 5A–C that the samples of (i) particle rein-forced composite could bear a load of 107 N with a com-pression of 1⋅23 mm, (ii) short fibre reinforced compositecould bear a load of 80 N with a compression of 1⋅24 mmand (iii) long fibre reinforced composite could bear a loadof 60 N with a compression of 1⋅25 mm, respectively.3.2d Wear test: As evident from figures 6A–C wearrate of UF matrix decreases appreciably when it is
Vijay Kumar Thakur and A S Singha262Figure 4. Compressive strength curves of P–Rnf/SF–Rnf and LF–Rnf composites (A, B and C).Figure 5. Flexural strength curves of P–Rnf/SF–Rnf and LF–Rnf composites (A, B and C).Figure 6. Wear resistance curves of P–Rnf/SF–Rnf and LF–Rnf composites (A, B and C).reinforced with Pine needles. It has been observed thatparticle reinforcement decreases the wear rate to a muchmore extent than short and long fibre reinforcements.From these results it is clear that these Pine needles areefficient candidates as reinforcing materials in UF matrixbased composites. This may be due to larger surface areaand more fibre/matrix interaction in case of Pine needlesreinforced polymer composites. Good interfacial strengthbetween the fibre and matrix is the most essential factorfor achieving good fibre reinforcement. The interfacialstrength depends on the surface topology of the fibre. Theinterface, therefore, plays a key role in controlling themechanical properties of a composite. Interfacial bondingis a result of good wetting of the fibres by the UF matrix
Natural fibres-based polymers 263Figure 7. SEM images of UF resin, P–Rnf, SF–Rnf and LF–Rnf composites (A, B, Cand D).Table 1. Thermogravimetric analysis of UF, PN and P–Rnf–UF composite.Sr. no. Sample code IDT (°C) % wt. loss FDT (°C) % wt. loss Final residue (%)1 PN 223 23⋅45 507 64⋅44 35⋅662 U–F resin 238 22⋅48 993 87⋅51 12⋅493 P–rnf–UF 235 27⋅51 805 69⋅63 29⋅37UF, Urea formaldehyde resin; PN, pine needles; P–Rnf, particle reinforced composite.Table 2. Differential thermal analysis of UF, PN and P–Rnf–UF composites.Sr. no. Sample code Exothermic/endothermic peaks, °C (μV)1 PN 333⋅2 (10⋅3); 478⋅1 (29⋅9)2 U–F resin 179 (6⋅8); 253 (5⋅7); 271 (27⋅9); 545 (9⋅4); 725 (–23⋅0)3 P–Rnf–UF 83 (2⋅7); 269 (23)UF, Urea formaldehyde resin; PN, pine needles; P–Rnf, particle reinforced composite.as well as the formation of a chemical bond between thefibre surface and the UF matrix. From the results ob-tained above we can conclude that different degrees ofreinforcement effects are achieved by the addition of Pineneedles to UF matrix based polymer. This may be dueto the different adhesion strengths between matrices andfibres. Particle reinforced composites show higher strengthdue to larger surface area and more fibre/matrix interaction.3.3 Morphological and thermal studies of biocompositesMorphological results obtained from SEM micrographs(figures 7A–D) clearly demonstrate that there is properintimate mixing of fibre with the resin in the compositesthus synthesized. It is clear from the micrographs thatthere is uniform mixing with particle reinforcement ascompared to short and long fibre reinforcements. Thermo-
Vijay Kumar Thakur and A S Singha264gravimetric analysis (TGA) of Pine needles, polymericUF resin and composites was investigated as a functionof % weight loss with the increase in temperature. In caseof raw fibre, in the beginning depolymerization, dehydra-tion and glucosan formation took place between the tempe-rature ranges of 26 and 195°C followed by the cleavageof C–H, C–C and C–O bonds. The initial decompositiontemperature (IDT) for pine needles has been found to be223°C and the final decomposition temperature (FDT) tobe 507°C as shown in table 1. On the other hand, in caseof UF resin it is single stage decomposition and theobserved initial decomposition temperature is 238°C andthe final decomposition of the resin took place at 993°C(table 1). It has been observed that for composites initialdecomposition temperature is 235°C and the final de-composition of the composite took place at 805°C (table1). These results are further supported by differentialthermal analysis (table 2). These values are between thedegradation temperatures observed for matrix and fibre.This indicates that the presence of cellulose fibres affectsthe degradation process of the biocomposites. Theseresults are consistent with the results reported earlier(Singha and Thakur 2008b).4. ConclusionsMechanical properties of randomly oriented intimatelymixed Pine needle reinforced UF composites were inves-tigated with special reference to the size of the fibre.Various test methods were used for complete mechanicalcharacterization of natural fibre reinforced composites. Incase of mechanical behaviour, particle reinforcement ofthe UF resin has been found to be more effective as com-pared to short and long fibre reinforcement. Themechanical behaviour has been strongly supported by theSEM analysis. Finally, it can be concluded that by utilizingPine needle, we can synthesize cost-effective and eco-friendly composite materials possessing suitable mecha-nical properties and this waste biomass can be a potentialcandidate for reinforcement in polymer composites.AcknowledgementsWe express our sincere thanks to the Director, NationalInstitute of Technology, Hamirpur, for providing basiclaboratory facilities. Financial assistance provided by theUniversity Grants Commission, New Delhi, through grantno. F. No. 30-80/2004 (SR) is highly acknowledged.ReferencesBledzki A K and Gassan J 1999 Prog. Polym. Sci. 24 221Chakraborty A, Sain M and Kortschot M 2006 ACS Symp.Series 938 169Chauhan G S, Bhatt S S, Kaur I, Singha A S and Kaith B S2000 J. Polym. Degrad. & Stab. 69 261Chauhan G S, Lal H, Singha A S and Kaith B S 2001 IndianJ. Fibre & Textile Res. 26 302Gassan J and Bledzki A K 1997 Compos. Part A–Appl. Sci. 281001Hornsby P R, Hinrichsen E and Tarverdi K 1997 J. Mater. Sci.32 1009Joshi S V, Drzal L T, Mohanty A K and Arora S 2004 Compo-sites: Part A 35 371Kaith B S and Kalia Susheel 2007 Int. J. Polym. Anal. & Charact.12 401Kaith B S, Singha A S and Kumar Kalia Susheel 2007 AUTEXRes. J. 7 119Mao L, Imam S, Gordon S, Cinelli P and Chiellini E 2000J. Polym. Environ. 8 205Mathew L, Joseph K U and Joseph R 2006 Bull. Mater. Sci. 2991Majumdar S and Adhikari B 2005 Bull. Mater. Sci. 28 703Misra B N, Kaur I, Gupta A, John V and Singha A S 1996Polym. Compos. 4 411Nakagaito A N and Yano H 2004 Appl. Phys. A – Mater. 78547Nakagaito A N and Yano H 2005 Appl. Phys. A – Mater. 80155Panthapulakkal S, Zereshkian A and Sain M 2006 BioresourceTechnol. 97 265Ray D, Sarkar B K, Rana A K and Bose N R 2001 Bull. Mater.Sci. 24 129Singha A S and Thakur Vijay K 2008a E-J. Chem. 5 782Singha A S and Thakur Vijay K 2008b Bull. Mater. Sci. 31791Singha A S, Kaith B S and Sarwade B D 2002 Hung. J. Ind.Chem. VESZPREM 30 289Singha A S, Kaith B S, Chauhan Ashish and Misra B N 2006J. Polym. Mater. 23 3456Singha A S, Shama Anjali and Thakur Vijay K 2008a Bull.Mater. Sci. 31 1Singha A S, Shama Anjali and Misra B N 2008b J. Polym.Mater. 25 91